guidelines for the blow molding of sarlink extrusion blow molding is the most widely used technique
Post on 13-Jun-2020
Embed Size (px)
Guidelines for the Blow Molding of Sarlink
The principles of blow molding 3 Introduction 3 Continuous extrusion blow molding 3 Multi-layer/sequentional co-extrusion blow molding 3 Injection blow molding 4 3D Blow molding 4 Suction blow molding 5 Press injection blow molding 5 Characteristics of the typical blow molding equipment for Sarlink 6 Screw design 6 Head and die design for continuous extrusion blow molding 6 Mold design 7 Shrinkage 7
Processing conditions for optimal blow molding of Sarlink 8 Drying and storage of Sarlink 8 Use of regrind 8 Coloring of Sarlink 8 Temperature settings 8 Blowing parameters 9 Maintenance of the equipment 9 Ancillary equipment 9
Appendix 1 10 Troubleshooting table for the extrusion blow molding of Sarlink
1 | Guidelines for the Blow Molding of Sarlink
In addition to standard types, a wide range of specialty grades are available, including high fl ow and UV stabilized grades.
Because of its combination of excellent fi nished part properties and easy processing, Sarlink thermoplastic vulcanizates have found many applications in a wide range of markets, including: automotive, building and construction, electrical, mechanical rubber goods, medical and leisure.
Sarlink thermoplastic vulcanizates are widely used in many blow molded parts such as rack & pinion steering gear boots, shock absorbers, strut covers, steering column cover, (3D sequential) automotive air ducts, cable ducts and many other applications in all market segments. This brochure is a guideline for the blow molding of Sarlink and shows an overview of the different blow molding techniques. A checklist for troubleshooting is available on the last pages.
Introduction Sarlink® thermoplastic vulcanizates (TPV) are based on dynamically vulcanized EPDM rubber particles dispersed in a polypropylene matrix.
Because of this morphology, Sarlink thermoplastic vulcanizates combine the performance characteristics of widely used thermoset rubbers, such as EPDM and polychloroprene, with the ease of plastic processing.
Sarlink offers a wide range of properties valuable to the end user. For instance: • resistance to high temperature • resistance to low temperature • excellent fl exural fatigue endurance • high impact strength • excellent resistance to chemicals and
solvents • excellent resistance to weathering • good electrical properties • high tear resistance • low tension and compression set • good resistance to oils (particularly harder
In addition to their superior performance characteristics, Sarlink thermoplastic vulcanizates, which are fully compounded, ready-to-use pellets, offer the following processing advantages compared to thermoset rubber: • no compounding • no vulcanization • low capital investment. • easy processing on standard thermoplastic
equipment for extrusion, injection molding and blow molding
• fast processing (short cycle times) • thermal stability/wide processing
window • low energy consumption • recycling of scrap generated during
processing • recycling of parts after service life • excellent control of product quality and
dimensional tolerances • in-line colorability • easy weldability (profi les, sheeting...) • material combinations by co-extrusion,
co-injection or co-blow molding to produce hard/soft articles, solid/sponge profi les...
2 | Guidelines for the Blow Molding of Sarlink
Extrusion blow molding is the most widely used technique. Sarlink is very suitable for blow molding because it has excellent melt strength and a high blow ratio. Sarlink gives a signifi cant weight reduction compared to thermoset rubber and Sarlink is fully recyclable. Table 1 shows an overview of application and material combinations.
The Principles of Blow Molding
Blow molding is the established technique for the production of hollow articles such as bellows and airducts. There are three major techniques for this process: • extrusion blow molding • press injection blow molding • injection blow molding.
Continuous extrusion blow molding
The principle of the extrusion blow molding process is that a parison, which is formed by continuous extrusion of material and rotating of the screw in the barrel, is clamped between two halves of a mold, cut-off and infl ated with air to fi ll the mold. The mold is cooled so that the product is frozen into the mold shape, while still under air pressure. The mold is then opened and the part removed. Due to the high melt stability and large blow-ratio (up to 4.5 for the high hardness grades) of Sarlink, large blow molded articles can be made. The processing steps are shown in fi gure 2.
Multi-layer/sequentional co-extrusion blow molding
Several polymers can be extruded in a multi-layer parison. The equipment is based on continuous extrusion or equipment with a melt accumulator. The thickness of each individual layer can be varied. Sarlink can be used in this kind of process to create e.g. a soft touch or rubber-like layer on polypropylene. The principles of the multi-layer extrusion blow molding system are shown in fi gure 1.
3 | Guidelines for the Blow Molding of Sarlink
Injection blow molding
The injection blow molding process is based on an injection molded preform instead of a directly extruded parison in the extrusion blow molding process. This process has the advantage of producing injection molded
The different materials can also be extruded sequentially. This is accomplished by reducing layer thickness to zero for one layer at a time in an alternating pattern. This technique is used to create hard-soft combinations. Automotive air ducts with fl exible ends and rigid pipe sections are produced with this process.
ends which have better control of dimensional tolerances. These machines are typically arranged in 3 or 4 stations that perform individual process steps. In the fi rst station the preform is injection molded. The machine is then indexed to the second position where the preform is infl ated into a blow molding cavity. In the third station the parts are ejected off the core rod. In the fourth station the core rods are tempered. This process is typically used to produce high production volume parts such as rack & pinion boots.
3D blow molding
This process is typically used for automotive air intake ducts. An advantage of three dimensional blow molding is that it is possible to make complex parts without generating fl ash along the edges. There are different techniques to make 3D articles. Figure 4a shows the process with a movable mold; fi gure 4b shows the movable head system on a fi xed mold. The parison can also be put into the mold by manipulating the parison with a robot.
4 | Guidelines for the Blow Molding of Sarlink
of the mold and the addition of a vacuum pump. One disadvantage of this system is the impossibility to produce complex 3D geometries. Another disadvantage is that the part diameter is limited. Figure 5 shows a simplifi ed representation of the suction blow molding system.
Press injection blow molding
Sarlink is an excellent material to use in a press injection blow molding system. This process is also known as the Ossberger process® , named after the equipment manufacturer. In this process the extruder initially fi lls a small
Suction blow molding
In this blow molding process the parison is sucked in the (closed) mold by a vacuum pump. This pump is connected to the bottom of the mold. The fi lling process of the mold takes place very rapidly (typically within a second). When the mold is fi lled, the parison is infl ated via an injected blow needle. This blow needle is injected on the top side of the parison.
The advantage of this blow molding technology is that it is possible to produce 3D blow molded parts on standard extrusion blow molding machines after a (small) change
injection mold which produces the end fi tting of the part. This mold is then lifted vertically while extruding a parison against the force of gravity. The wall thickness is adjusted during the extrusion process by varying the die gap. The mold closes around the injection mold and the parison, and the parison is blown into the mold cavity. The mold opens and the part is removed for trimming. The principle of this press injection blow-molding system is shown in fi gure 6.
®Registered trade name of Ossberger- Turbinenfabrik GmbH & Co.
5 | Guidelines for the Blow Molding of Sarlink
Mixing pins or shear segments are often used with general purpose screws to improve melt homogeneity and dispersion of colorants and additives.
Barrier screws The use of a low shear barrier screw will provide the higher throughput and improved melt quality. A generous barrier clearance is used (typically 1.5 to 2.0 mm). The barrier section should be followed with a Maddock mixing section to further homogenize the melt. Consult DSM for further design recommendations regarding barrier screws.
Head and die design for continuous extrusion blow molding
Head design. Polyolefi n head designs are also recommended for Sarlink. Important factors in head design are: •